6168 J. Phys. Chem. A 2003, 107, 6168-6175On the Electronic and Atomic Structures of Small Au N - (N ) 4-14) Clusters:A Photoelectron Spectroscopy and Density-Functional StudyHannu Ha1kkinen,* Bokwon Yoon, and Uzi LandmanSchool of Physics, Georgia Institute of Technology, Atlanta, Georgia 30332Xi Li, Hua-Jin Zhai, and Lai-Sheng WangDepartment of Physics, Washington State UniVersity, 2710 UniVersity DriVe, Richland, Washington 99352, andW. R. Wiley EnVironmental Molecular Sciences Laboratory, Pacific Northwest National Laboratory, MS K8-88,P.O. Box 999, Richland, Washington 99352ReceiVed: May 23, 2003; In Final Form: June 24, 2003We report a joint experimental and theoretical study of the electronic and atomic structures of small goldclusters with up to 14 atoms. Well-resolved photoelectron spectra were obtained for Au N- (N ) 1-14) atseveral photon energies. Even-odd alternations were observed, where the even-sized clusters (except Au 10- )exhibit an energy gap between the lowest binding energy peak and the rest of the spectrum, indicating thatall the neutral even-sized clusters have closed shells. The Au 10- spectrum reveals the existence of isomers,with the ground-state cluster exhibiting an extremely high electron binding energy. Evidence of multipleisomers was also observed in the spectra of N ) 4, 8, 12, and 13. The structures of the gold cluster anionsin the range N ) 4-14 were investigated using first-principles simulations. A striking feature of the anionicclusters in this range is the occurrence of planar ground-state structures, which were predicted in earliertheoretical studies (Häkkinen, H.; et al. Phys. ReV. Lett. 2002, 89, 033401) and observed in ion-mobilityexperiments (Furche, F.; et al. J. Chem. Phys. 2002, 117, 6982) and the existence of close-lying isomers. Thecalculated electron detachment energies and density of states were compared with the measured data, whichconfirmed the ground-state structures of the anions. It is found that the main isomers observed experimentallyindeed consist of planar clusters up to Au 12- , whereas for Au 13- and Au 14- the theoretical results from threedimensionalisomers agree better with the experiment, providing further support for the 2D to 3D structuraltransition at Au 12- , as concluded from previous ion mobility experiments. We also find that small neutralclusters exhibit a tendency to form two-dimensional structures up to a size of 13 atoms.I. IntroductionThe recent surge of research activity in the area of the physicaland chemical properties of gold clusters and nanoparticles ismotivated by their potential applications as building blocks forfunctional nanostructured materials, electronic devices, andnanocatalysts. 1-27 An added interest was created by the mostrecent experimental and theoretical discoveries of large (up toabout 12 atoms) planar gas-phase anionic gold clusters. 17,18 Theoccurrence of planar metal clusters of this size is unprecedented,and their stability was explained by, and attributed to, 18 strongrelativistic bonding effects 28 in gold that reduce the s-d energygap, thus inducing hybridization of the atomic 5d-6s levelsand causing overlap of the 5d shells of neighboring atoms inthe cluster.We report here a systematic combined high-resolution photoelectronspectroscopy and density-functional investigation ofthe atomic and electronic structure of gold cluster anions Au N-with N ) 1-14. This study is complementary in many ways tothe ones reported previously. First, it provides photoelectronspectra (PES) with much better resolution than the previousworks 2,3 enabling identification of several new important features* Corresponding author. Current address: Department of Physics,FIN - 40014 University of Jyväskylä, Finland. E-mail: Hannu.Hakkinen@phys.jyu.fi.due to isomers in the cluster beam. Second, our densityfunctionalcalculations extend the range of those reported byus before, 12,18 including a critical examination of several clusterisomers for each cluster size. Finally, comparison of ourcalculated results with the experiments reported here allows usto assign the probable ground-state structures and the importantisomers existing in the cluster beam, providing the basicstructural information for future studies of the physics andchemistry of these systems. 18The paper is organized as follows. Brief descriptions of theexperimental and theoretical methods used in this study are givenin sections II and III. The experimental results are presented insection IV, and section V gives the theoretical results and adiscussion of the comparison between the theoretical predictionsand the measured data. We summarize our results in sectionVI.II. Experimental DetailsThe experiments were performed using a magnetic-bottlephotoelectron apparatus equipped with a laser vaporizationcluster source. 29,30 A pure gold disk target was ablated by apulsed laser beam (10 mJ/pulse at 532 nm). The laser-inducedplasma was mixed with a helium carrier gas delivered by apulsed valve at a backing pressure of 10 atm. The clustersformed in the nozzle were entrained with the carrier gas and10.1021/jp035437i CCC: $25.00 © 2003 American Chemical SocietyPublished on Web 07/23/2003
Structures of Small Au N - (N ) 4-14) Clusters J. Phys. Chem. A, Vol. 107, No. 32, 2003 6169underwent a supersonic expansion. After passing a skimmer,negatively charged gold clusters were extracted from thecollimated cluster beam perpendicularly and subjected to a timeof-flightmass analysis. A given cluster of interest was massselectedand decelerated before photodetachment by an ArFexcimer laser (193 nm) or a Nd:YAG laser (266 and 355 nm).Photoelectrons were measured using a magnetic-bottle timeof-flightanalyzer and calibrated by the known spectra of Au -and Rh - . Care was taken to produce relatively cold clusters,which are essential to yield highly resolved photoelectronspectra. 31,32 The experimental resolution (∆E/E) was ∼2.5%,i.e., ∼25 meV for 1 eV electrons.III. Computational MethodsThe electronic and geometric structures of the gold clusteranions were obtained through Born-Oppenheimer (BO) localspin-density-functional (LSD) molecular dynamics (MD) simulations(BO-LSD-MD) 33 employing norm-conserving scalarrelativisticpseudopotentials 34 for the 5d 10 6s 1 valence electronsof the gold atom, with self-consistent gradient corrections (PBE-GGA). 35 The Kohn-Sham (KS) orbitals were expanded in aplane-wave basis with a 62 Ry kinetic energy cutoff. Thisapproach has been used by us in numerous occasions previouslyand its feasibility and accuracy for gold has been welldocumented. 12,14,18 The BO-LSD-MD method is particularlysuited for studies of finite charged systems because it does notemploy a supercell (periodic replication of the atoms), thusallowing for accurate determination of the total energy of bothcharged and neutral systems and the corresponding electronremoval (detachment) energies. All the clusters were relaxedfully without any symmetry constraints. A large number of initialstructural candidates were used, but here we report only thefew energetically lowest-lying isomers for each size, which areimportant in interpreting the experimental data.IV. Experimental Photoelectron SpectraThe photoelectron spectra for Au - N (N ) 1-14) are shownin Figures 1 and 2 at 193 nm (6.424 eV) and 266 nm (4.661eV), respectively. A few selected clusters with lower electronbinding energies were also investigated at 355 nm (3. 496 eV),as shown in Figure 3, where only the threshold peak wasobserved in each case. The spectra were all highly resolved withnumerous discrete electronic transitions up to the highest photonenergy used (6.424 eV).A. 193 nm Spectra. The current data at 193 nm are consistentwith the previous data measured at 157 nm (ref 2) but are muchbetter resolved. Our spectra for Au - 2 to Au - 4 at 193 nm werealso consistent with a previous study at the same photon energy,except for the peak at 6.26 eV for Au - 2 , which was not observedin the previous work. 3 The most significant feature in the spectrais the even-odd alternation, where the even clusters show lowerelectron binding energies and a sizable energy gap (betweenthe lowest-binding-energy peak and the rest of the spectrum),indicating that the neutral even-sized clusters are closed-shellelectronic systems. The largest energy gap was observed in thespectrum of Au - 6 : 2.34 eV, which is in fact the largest amongall the coinage metal clusters, even larger than the 1.8 eV gaprecently found in the tetrahedral Au 20 . 25However, the spectrum of Au - 10 represents a clear exceptionto the even-odd pattern. The weak signals in the lower bindingenergy range between 2.6 and 3.8 eV of the Au - 10 spectrumwere actually due to weakly populated isomers. In fact, thevertical binding energy (VDE) of the main isomer of Au- 10was measured to be 3.92 eV, higher than that of either Au- 9Figure 1. Photoelectron spectra of Au N- (N ) 1-14) measured at193 nm (6.424 eV).(3.84 eV) or Au 11 - (3.80 eV). Minor isomers were also observedfor other clusters, notably in the spectrum of Au 4 - , where twoweak features were observed in the HOMO-LUMO gap regionat VDEs of 3.41 and 3.76 eV. A very weak peak at 2.49 eV inthe Au 4 - spectrum should also come from an isomer. In thespectra of Au 8 - and Au 12 - , the first peak showed a splitting,each with a shoulder on the higher energy side. The splitting istoo large to be attributed to vibrational excitations and it is likelydue to the presence of isomers with similar VDEs as the mainisomers. The weak feature at the lowest energy side (3.76 eV)in the spectrum of Au 13 - is also indicative of a contributionfrom a minor isomer. As will be shown later, all the observedisomers are indeed born out from the accompanying theoreticalcalculations.B. 266 and 355 nm Spectra. The spectra at 266 nm weremuch better resolved for the low binding energy featuresaccessible at this photon energy (Figure 2). In particular, theweak features attributed to anion isomers in the spectra of Au 4 - ,Au 8 - ,Au 10 - ,Au 12 - , and Au 13 - can be seen more clearly. Thespectrum of Au 3 - exhibited the most dramatic dependence onthe photon energy: the relative intensities of the first two peaks(VDEs: 3.88 and 4.39 eV) were similar at 193 nm, but therelative intensity of the 4.39 eV peak was significantly reducedat 266 nm. The 3.88 eV peak of Au 3 - was extremely sharp, itswidth (40 meV fwhm) was close to the instrumental resolution,indicating that there is no geometry change between the anionand the neutral ground states for the gold trimer.The spectra of other clusters did not display much photonenergy dependence, except the surprising observation of continuouselectron signals in the HOMO-LUMO gap region inthe spectra of Au 12 - and Au 14 - . Similar signals were alsoobserved as a higher binding energy tail in the spectra of Au 6-
6170 J. Phys. Chem. A, Vol. 107, No. 32, 2003 Häkkinen et al.Figure 3. Photoelectron spectra of Au N- (N ) 6, 7, 8, 12, 14) measuredat 355 nm (3.496 eV).Figure 2. Photoelectron spectra of Au N- (N ) 1-14) measured at266 nm (4.661 eV).and Au 8 - . To a lesser degree, the tails were also present in the266 nm spectra of Au 7 - ,Au 9 - , and Au 11 - . These signals seemedto be continuous and featureless; they were not due to contributionsfrom isomers. These signals exhibited no photon fluxdependence, but depended on the detachment photon energiesbecause they were not observed in the 193 nm spectra. Theyappeared to be due to delayed detachment, analogous to delayedionization observed for neutral clusters. 36 It seemed that theparent anion was capable of absorbing a photon to create atemporarily excited anion, which then autodetached. Thisabsorption might be due to the plasma resonance of the anionicclusters. Plasma resonance has been observed in neutral andcationic alkali and coinage clusters, 37,38 though none has beenreported for anionic clusters.We only obtained spectra at 355 nm for a few selected clusters(Figure 3). We were particularly interested in resolving thesplittings of the two features in the spectra of Au 8 - and Au 12 - .Unfortunately, the delayed detachment signals were sufficientlystrong to wash out the weaker feature on the higher energy side.It turned out that these features were better observed in the 266nm spectra (Figure 2). The second feature was observed to haveVDEs of 2.93 and 3.22 eV, compared to the main feature at2.79 and 3.06 eV for Au 8 - and Au 12 - , respectively.C. Adiabatic and Vertical Detachment Energies. TheVDEs for each cluster anion can be easily determined from thepeak maximum in each spectrum. The adiabatic detachmentenergies (ADEs), which also represent the electron affinities(EAs) of the corresponding neutral clusters, were more difficultto measure without vibrational resolution. We estimated theADEs by drawing a straight line at the leading edge of theground-state feature and then adding a constant to the intersectionswith the binding energy axis to account for the instrumentalresolution. Although this is an approximate procedure, we wereable to obtain consistent ADEs from spectra taken at differentphoton energies, due to the relative sharp onset of the data. Allthe ADEs were determined from the 266 nm spectra or the 355nm spectra, when available. More accurate ADEs were obtainedin the lower photon energy spectra because of the better resolvedfeatures. The obtained ADEs and VDEs are listed in Table 1.V. Theoretical Results and DiscussionA. Low-Energy Structures and Detachment Energies. Anumber of optimized low-energy structures for Au - N , with N) 4-14, are shown in Figure 4 and their structural and energeticcharacteristics are summarized in Table 1. A striking feature inFigure 4 is the occurrence of energetically favorable planarstructures up to Au - 14 (for clusters larger than Au - 10 , manylow-lying 3D isomers appear but the ground-states predictedby DFT are still strictly planar). This phenomenon is unique togold clusters and is related to strong relativistic effects in theirbonding, which lead to enhanced s-d hybridization and d-dinteraction, as was discussed recently by some of us. 18 Recention mobility experiments and related DFT calculations also yieldsupport for large planar gold anions 17 up to about N ) 12 (forN ) 12 two distinct mobilities were detected and assigned to acoexistence of both planar and 3D structures).Figure 5 shows the comparison of the calculated andmeasured VDEs. For most clusters, the theoretical ground-stateVDE value (filled dot) is within 5-6% of the experimentalresult. For N ) 4 and 14, the best agreement with experimentis obtained not for the ground-state structure, but rather forcertain low-lying isomers. This indicates that even though thehigh resolution of the experimental PES data implies that thetemperature of the cluster beam is low (in a previous study ofanionic aluminum clusters in a similar setup the minimum
Argosy University Distance Learning Information forStudentsOnline LearningPlatformArgosy University uses the eCollege platform for online and blendedcourses. Some face-to-face courses may also use eCollege to shareinformation electronically.AccessingeCollege throughthe ArgosyUniversityStudent PortaleCollegeTechnicalRequirementseCollegeStudentOrientationCourse1. Go to the Argosy Student Portalat http://mycampus.argosy.eduand enter your Student Portallogin and password; click theLogin button.2. On the portal homepage, lookfor the My Classes section onthe right side of the screen.Click the course title link toaccess your online classroom directlyorClick the red “Go to my classes” button locate your courses in theeCollege Course List. Click the blue title link to enter the course.You will have access to your courses 3-days before the first day ofa session.1. Go to http://myeclassonline.com; click “NO” on the pop up window2. Click “Technical Requirements”; click “NO” on the pop up windowIt is highly recommended that you complete an eCollege tutorialbefore starting courses. To access the tutorial, click on the red “Go tomy classes” button in the student portal 2 weeks before the sessionstarts. This orientation course will remain in your account until youcomplete your program.ParticipationYou must login and participate in their eCollege course on a weeklybasis. Please see your course syllabus for additional information.TextbooksIf your course is using an eBook, the link to your book will be availablein your eCollege course.If your course is using a printed textbook, your book will be availableat the MBS Direct online bookstore: http://direct.mbsbooks.com/argosy.htmOnlineClassroomSupportoooContact the Student Technical Help Desk for support usingthe Student Portal, online eCollege classroom, Argosy DigitalBookshelf and eBooks, or student email at 1.866.4.ARGOSY(1.866.427.4679)Contact your instructor for questions about course requirements.Contact your campus if you believe you are enrolled in the wrongclass or section.Updated: March 20106
6174 J. Phys. Chem. A, Vol. 107, No. 32, 2003 Häkkinen et al.Figure 12. Same as Figure 6 but for structures 12A-12C of Au 12- .Figure 13. Same as Figure 6 but for structures 14A and 14B of Au 14- .The VDE of the first isomer, 2.94 eV, matches the first weakPES feature at 2.9 eV.Au 12 - . Our calculations predict the planar D 3h structure 12Ato be a clear ground state, followed by a planar C 2h structure12B and a 3D C 2V structure 12C. The DOS spectra of all theseclusters have a clear HOMO-LUMO gap, of the order of 0.8eV, separating the first two peaks (Figure 12). This agrees wellwith the experimental PES spectra (Figures 1 and 2), whichrevealed a HOMO-LUMO gap of about 0.9 eV. On the basisof the comparison between the measured and calculated mobilityparameters for clusters 12A and 12C, Kappes et al. 17 concludedthat N ) 12 is the critical size for the 2D-3D transition, namelyisomers of both dimensionality are present in the Au 12 - anionbeam, and clusters with N > 12 are three-dimensional. Thecomparison of our calculated VDE values (12A, 3.24 eV; 12B,3.25 eV; 12C, 3.10 eV) agree well with the measured value of3.06 eV. Additionally, the contributions from all these clusterswould give a double feature in the first photodetachment peak,as is indeed observed experimentally. Thus, our work givesfurther support for the conclusion of ref 17 that both planarand 3D structures are present in the beam of Au 12 - .Au 14 - . For the cluster anions we found two structures, 14Aand 14B, within an energy interval of 0.1 eV, with significantlydifferent DOS features (Figure 13). The experimental datarevealed a large HOMO-LUMO gap of 1 eV, which is wellreproduced by the three-dimensional cagelike structure 14B(1.05 eV), as well as the calculated singlet-triplet separation(see discussion for N ) 6 above) ∆E N S-T ) 1.07 eV. Keepingin mind the inherent accuracy of the DFT (of the order of 0.1eV), as well as the previously reported tendency of DFT toslightly overestimate the stability of planar structures, we assertthat the experimental PES for N ) 14 indicates the predominanceof 3D clusters, and the most likely candidate is structure14B predicted from our calculation. This conclusion is alsoconsistent with that extracted from analysis of ion mobilityexperiment that above N ) 12, three-dimensional gold clusteranions become more stable.C. Energetics and Dimensionality of the Neutral ClustersAu N , N ) 4-14. The last column in Table 1, marked by “O n ”,indicates the energy ordering of the neutral Au N clusters as theyare relaxed from the corresponding anionic cluster after electrondetachment, utilizing the calculated information about the energydifference of various anionic cluster isomers and their adiabaticelectron detachment energies. As can be seen, for most clustersizes the energetic ordering of the neutral clusters does notfollow that of the corresponding anions. It is intriguing to notethat the planar structures are energetically very competitive withrespect to 3D structures also in neutral gold clusters; indeed,only for the largest size considered, Au 14 , we have found a 3Dground-state structure. Although our theoretical predictionsindicate that also neutral gold clusters favor planar structuresup to unprecedented large sizes, experimental verification ofthis result is complicated because the cluster beam experimentusually observes properties of charged clusters. For singlepositively charged gold clusters Au N + the 2D-3D transitionsize has been deduced to be N ) 8 in the ion mobilityexperiment. 41 Our current theoretical predictions indicate thatit should be interesting to study the 2D-3D crossover sizeexperimentally for neutral gold clusters deposited on weak andsmooth substrates, such as an ideal graphite surface.VI. SummaryIn this work, well-resolved photoelectron spectra and scalarrelativisticDFT calculations are reported for anionic goldclusters with 1-14 atoms. The combined experimental andtheoretical investigation allows us to gain insight into thestructural characteristic and growth patterns of the cluster anionsand make tentative assignments of the PES features.In general, we find that the most likely structural candidatesfor clusters up to N ) 12 are planar, confirming the findingsobtained by Kappes and co-workers 17 from analysis of theirmobility experiments. For N ) 13, a definite structural assignmentcannot be done on the basis of the PES data, due to theexistence of many low-lying 2D and 3D isomers. For N ) 14,a 3D cagelike structure has been assigned. Isomeric effects arerecognizable in the experimental PES data for several clustersizes, most notably for N ) 4, 7, 8, 10, and 12. The 2D-3Dtransition seems to take place via cagelike structures, but for N) 13 the commonly considered icosahedral or cuboctahedralstructures are not energetically favorable. This work providesboth geometric structural information and characteristics of theelectronic structure, which gives the impetus for further theoreticalinvestigations of the physics and chemistry of small gasphasegold clusters.Acknowledgment. The experimental work was supportedby the National Science Foundation (CHE-9817811) andperformed at the W. R. Wiley Environmental MolecularSciences Laboratory, a national scientific user facility sponsoredby DOE’s Office of Biological and Environmental Researchand located at Pacific Northwest National Laboratory, which isoperated for DOE by Battelle under Contract DE-AC06-76RLO1830. The theoretical work was supported by the U.S. AFOSRand partially (H.H.) by the Academy of Finland. The computa-
Structures of Small Au N - (N ) 4-14) Clusters J. Phys. Chem. A, Vol. 107, No. 32, 2003 6175tions were performed at NERSC, CA, and in the Center forComputational Materials Science at the Georgia Institute ofTechnology.References and Notes(1) Cox, D. M.; Brickman, R.; Creegan, K.; Kaldor, A. Z. Phys. D1991, 19, 353. Cox, D. M.; Brickman, R.; Creegan, K. A. Mater. Res. Soc.Symp. Proc. 1991, 206, 34.(2) Taylor, K. J.; Pettiette-Hall, C. L.; Cheshnovsky, C.; Smalley, R.E. J. Chem. Phys. 1992, 96, 3319.(3) Handschuh, H.; Gantefor, G.; Bechthold, P. S.; Eberhardt, W. J.Chem. Phys. 1994, 100, 7093.(4) Lee, T. H.; Ervin, K. M. J. Phys. Chem. 1994, 98, 10023.(5) Haruta, M. Catal. Today 1997, 36, 153.(6) Valden, M.; Lai, X.; Goodman, D. W. Science 1998, 281, 1647.(7) Garzon, I. L.; Michaelian, K.; Beltrán, M. R.; Posada-Amarillas,A.; Ordejón, P.; Artacho, E.; Sánchez-Portal, D.; Soler, J. M. Phys. ReV.Lett. 1988, 81, 1600.(8) Häkkinen, H.; Barnett, R. N.; Landman, U. Phys. ReV. Lett. 1999,82, 3264.(9) Sanchez, A.; Abbet, S.; Heiz, U.; Schneider, W.-D.; Häkkinen, H.;Barnett, R. N.; Landman, U. J. Phys. Chem. A 1999, 103, 9573.(10) Bond, G. C.; Thompson, D. T. Catal. ReV.-Sci. Eng. 1999, 41,319.(11) Salisbury, B. E.; Wallace, W. T.; Whetten, R. L. Chem. Phys. 2000,262, 131.(12) Häkkinen, H.; Landman, U. Phys. ReV. B2000, 62, R2287.(13) Grönbeck, H.; Andreoni, W. Chem. Phys. 2000, 262, 1.(14) Häkkinen, H.; Landman, U. J. Am. Chem. Soc. 2001, 123, 9704.(15) Hagen, J.; Socaciu, L. D.; Elijazyfer, M.; Heiz, U.; Bernhardt, T.M.; Wöste, L. Phys. Chem. Chem. Phys. 2002, 4,1707.(16) Wallace, W. T.; Whetten, R. L. J. Am. Chem. Soc. 2002, 124, 7499.(17) Furche, F.; Ahlrichs, R.; Weis, P.; Jacob, C.;. Gilb, S.; Bierweiler,T.; Kappes, M. J. Chem. Phys. 2002, 117, 6982.(18) Häkkinen, H.; Moseler, M.; Landman, U. Phys. ReV. Lett. 2002,89, 033401. The planar ground-state structures of Au - N , N e 13, were firstreported in footnote 28 of this paper. The close similarity of the structuresand the isomeric order of the low-lying cluster isomers found in the currentwork and in ref 17 is encouraging and reassuring in light of the differentpseudopotentials, basis sets, and exchange-correlation functionals used inthese two independent calculations.(19) Mills, G.; Gordon, M. S.; Metiu, H. Chem. Phys. Lett. 2002, 359,493.(20) Boyen, H.-G.; Kästle, G.; Weigl, F.; Koslowski, B.; Dietrich, C.;Ziemann, P.; Spatz, J. P.; Riethmüller, S.; Hartmann, C.; Möller, M.; Schmid,G.; Garnier, M. G.; Oelhafen, P. Science 2002, 297, 1533.(21) Pyykkö, P.; Runeberg, N. Angew. Chem. Int. Ed. 2002, 41, 2174.(22) Li, X.; Kiran, B.; Li, J.; Zhai, H.-J.; Wang, L.-S. Angew. Chem.Int. Ed. 2002, 41, 4786.(23) Häkkinen, H.; Abbet, S.; Sanchez, A.; Heiz, U.; Landman, U.Angew. Chemie Int. Ed. 2003, 42, 1297.(24) Mills, G.; Gordon, M. S.; Metiu, H. J. Chem. Phys. 2003, 118,4198.(25) Li, J.; Li, X.; Zhai, H.-J.; Wang, L.-S. Science 2003, 299, 864.(26) Yoon, B.; Häkkinen, H.; Landman, U. J. Phys. Chem. A 2003, 107,4066.(27) Socaciu, L. D.; Hagen, J.; Bernhardt, T. M.; Wöste, L.; Heiz, U.;Häkkinen, H.; Landman, U. Submitted for publication to J. Am. Chem. Soc.(28) Pyykkö, P. Chem. ReV. 1988, 88, 563.(29) Wang, L. S.; Cheng, H. S.; Fan, J. J. Chem. Phys. 1995, 102, 9480.(30) Wang, L. S.; Wu, H. In AdVances in Metal and SemiconductorClusters. IV. Cluster Materials; Duncan, M. A., Ed.; JAI Press: Greenwich,1998; pp 299-343.(31) Akola, J.; Manninen, M.; Häkkinen, H.; Landman, U.; Li, X.; Wang,L. S. Phys. ReV. B1999, 60, R11297.(32) Wang, L. S.; Li, X. In Proceedings of the International Symposiumon Clusters and Nanostructure Interfaces (Oct. 25-28, 1999, Richmond,VA); Jena, P., Khanna, S. N., Rao, B. K., Ed.; World Scientific: RiverEdge, NJ, 2000; pp 293-300.(33) Barnett, R. N.; Landman, U. Phys. ReV. B1993, 48, 2081.(34) Troullier, N.; Martins, J. L. Phys. ReV. B 1991, 43, 1993.(35) Perdew, J. P.; Burke, K.; Ernzerhof, M. Phys. ReV. Lett. 1996, 77,3865.(36) Haufler, R. E.; Wang, L. S.; Chibante, L. P. F.; Jin, C.; Conceicao,J.; Chai, Y.; Smalley, R. E. Chem. Phys. Lett. 1991, 179, 449.(37) Amrein, A.; Simpson, R.; Hackett, P. J. Chem. Phys. 1991, 94,4663.(38) Bréchignac, C.; Cahuzac, P.; Kebaïli, N.; Leygnier, J. Sarfati, A.;Phys. ReV. Lett. 1992, 68, 3916.(39) Tozer, D. J.; Handy, N. C. J. Chem. Phys. 1998, 108, 2545; J.Chem. Phys. 1998, 109, 10180.(40) Taylor, K. J.; Jin, C.; Conceicao, J.; Wang, L.-S.; Cheshnovsky,O.; Johnson, B. R.; Nordlander, P. J.; Smalley, R. E. J. Chem. Phys. 1990,93, 7515.(41) Gilb, S.; Weis, P.; Furche, F.; Ahlrichs, R.; Kappes, M. M. J. Chem.Phys. 2002, 116, 4094.